LMucko/crystallography-open-database huggingface dataset:
Dati strutturali sulla tarbuttite
Fanfani, L.; Zanazzi, P. F.; Periodico di Mineralogia 34 (1965) 539–545; doi:

data_9016204
_publ_section_title
;
 Dati strutturali sulla tarbuttite
;
_journal_name_full               'Periodico di Mineralogia'
_journal_page_first              539
_journal_page_last               545
_journal_volume                  34
_journal_year                    1965
_chemical_compound_source        'Broken Hill, Rhodesia'
_chemical_formula_sum            'H O5 P Zn2'
_chemical_name_mineral           Tarbuttite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                102.85
_cell_angle_beta                 102.77
_cell_angle_gamma                86.83
_cell_formula_units_Z            2
_cell_length_a                   5.499
_cell_length_b                   5.654
_cell_length_c                   6.465
_cell_volume                     191.120
_database_code_amcsd             0014936
_exptl_crystal_density_diffrn    4.218
_cod_original_formula_sum        'Zn2 P O5 H'
_cod_database_code               9016204
Structure du tris(chromato)arsenate de diammonium-hydrogene, (NH4)2HCr3AsO13: mise en evidence d'un nouvel anion (Cr3AsO13)^3-^
Averbuch-Pouchot, M. T.; Acta Crystallographica, Section B 34 (1978) 3350–3351; doi:10.1107/S0567740878010894

data_9016205
_publ_section_title
;
 Structure du tris(chromato)arsenate de diammonium-hydrogene, (NH4)2HCr3AsO13:
 mise en evidence d'un nouvel anion (Cr3AsO13)^3-^
;
_journal_issue                   11
_journal_name_full               'Acta Crystallographica, Section B'
_journal_page_first              3350
_journal_page_last               3351
_journal_paper_doi               10.1107/S0567740878010894
_journal_volume                  34
_journal_year                    1978
_chemical_formula_sum            'As Cr3 N2 O13'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 93.12
_cell_angle_gamma                90
_cell_length_a                   14.02
_cell_length_b                   9.49
_cell_length_c                   9.57
_cell_formula_units_Z            4
_cell_volume                     1271.399
_database_code_amcsd             0015979
_exptl_crystal_density_diffrn    2.439
_cod_duplicate_entry             1008032
_cod_original_formula_sum        'N2 As Cr3 O13'
_cod_database_code               9016205
_amcsd_formula_title             (NH4)2HCr3AsO13
The crystal structure of the natural strontium borate, p-veatchite, Sr2[B5O8(OH)]2*B(OH)3*H2O Note: polytype veatchite-1M, formally known as veatchite-p
Rumanova, I. M.; Gandymov, O.; Soviet Physics Crystallography 16 (1971) 75–81; doi:

data_9016206
_publ_section_title
;
 The crystal structure of the natural strontium borate, p-veatchite,
 Sr2[B5O8(OH)]2*B(OH)3*H2O
 Note: polytype veatchite-1M, formally known as veatchite-p
;
_journal_name_full               'Soviet Physics Crystallography'
_journal_page_first              75
_journal_page_last               81
_journal_volume                  16
_journal_year                    1971
_chemical_compound_source        'Inderskii formation, Kazakh SSR'
_chemical_formula_sum            'B11 H7 O22 Sr2'
_chemical_name_mineral           Veatchite
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 119.25
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.70
_cell_length_b                   20.80
_cell_length_c                   6.60
_cell_volume                     802.501
_database_code_amcsd             0018907
_exptl_crystal_density_diffrn    2.703
_cod_original_formula_sum        'Sr2 B11 O22 H7'
_cod_database_code               9016206
Synthese et structure crystalline d'un nouvel oxyde mixte "FeV3O8" (Fex V1-x O2; x=approximately 0.25) _cod_database_code 1008165
Muller, J.; Joubert, J.; Marezio, M.; Journal of Solid State Chemistry 27 (1979) 191–199; doi:10.1016/0022-4596(79)90157-9

data_9016207
_publ_section_title
;
 Synthese et structure crystalline d'un nouvel oxyde mixte "FeV3O8"
 (Fex V1-x O2; x=approximately 0.25)
 _cod_database_code 1008165
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              191
_journal_page_last               199
_journal_paper_doi               10.1016/0022-4596(79)90157-9
_journal_volume                  27
_journal_year                    1979
_chemical_formula_sum            'Fe0.5 O4 V1.5'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 106.85
_cell_angle_gamma                90
_cell_length_a                   12.129
_cell_length_b                   3.679
_cell_length_c                   6.547
_cell_formula_units_Z            4
_cell_volume                     279.601
_database_code_amcsd             0016105
_exptl_crystal_density_diffrn    3.999
_cod_duplicate_entry             1008165
_cod_original_formula_sum        'Fe.5 V1.5 O4'
_cod_database_code               9016207
_amcsd_formula_title             'Fe O8 V3'
Crystal structure and magnetic ordering in Er Fe6 Ge6 studied by X-ray, neutron diffraction and magnetic measurements _cod_database_code 1006126
Oleksyn, O.; Schobinger-Papamantellos P; Rodriguez-Carvajal J; Brueck, E.; Buschow, K.; Journal of Alloys and Compounds 257 (1997) 36–45; doi:

data_9016208
_publ_section_title
;
 Crystal structure and magnetic ordering in Er Fe6 Ge6 studied by X-ray,
 neutron diffraction and magnetic measurements
 _cod_database_code 1006126
;
_journal_name_full               'Journal of Alloys and Compounds'
_journal_page_first              36
_journal_page_last               45
_journal_volume                  257
_journal_year                    1997
_chemical_formula_sum            'Er0.5 Fe3 Ge2.987'
_space_group_IT_number           71
_symmetry_space_group_name_Hall  '-I 2 2'
_symmetry_space_group_name_H-M   'I m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0991
_cell_length_b                   26.5293
_cell_length_c                   5.10721
_cell_formula_units_Z            12
_cell_volume                     1097.353
_database_code_amcsd             0012793
_exptl_crystal_density_diffrn    8.499
_cod_duplicate_entry             1006126
_cod_original_formula_sum        'Er.5 Ge2.987 Fe3'
_cod_database_code               9016208
_amcsd_formula_title             'Er Fe6 Ge6'
Polymorphism of donnayite (Na,TR)Sr(CO3)2*H2O
Tjy, C. T. L.; Pobedimskaya, E. A.; Nadezhina, T. N.; Khomyakov, A. P.; Moscow University Geology Bulletin 47 (1992) 60–70; doi:

data_9016209
_publ_section_title
;
 Polymorphism of donnayite (Na,TR)Sr(CO3)2*H2O
;
_journal_name_full               'Moscow University Geology Bulletin'
_journal_page_first              60
_journal_page_last               70
_journal_volume                  47
_journal_year                    1992
_chemical_compound_source        'Khibiny alkaline massif'
_chemical_formula_sum
'C2 H2 Ba0.09 Ca0.19 Ce0.11 Dy0.02 Er0.01 Gd0.02 La0.09 Na0.5 O7 Pr0.01 Sr0.71 Y0.24 Yb0.01'
_chemical_name_mineral           Donnayite-(Y)
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.211
_cell_length_b                   5.211
_cell_length_c                   18.357
_cell_volume                     431.692
_database_code_amcsd             0018482
_exptl_crystal_density_diffrn    3.372
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum
'Na.5 Y.24 Ce.11 La.09 Gd.02 Dy.02 Er.01 Yb.01 Pr.01 Sr.71 Ca.19 Ba.09 C2 O7 H2'
_cod_database_code               9016209
Structure du germanate d'hafnium
Durif, A.; Acta Crystallographica 14 (1961) 312–312; doi:10.1107/S0365110X61000942

data_9016210
_publ_section_title
;
 Structure du germanate d'hafnium
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica'
_journal_page_first              312
_journal_page_last               312
_journal_paper_doi               10.1107/S0365110X61000942
_journal_volume                  14
_journal_year                    1961
_chemical_formula_sum            'Ge Hf'
_space_group_IT_number           88
_symmetry_space_group_name_Hall  'I 4bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.849
_cell_length_b                   4.849
_cell_length_c                   10.501
_cell_formula_units_Z            4
_cell_volume                     246.908
_database_code_amcsd             0009248
_exptl_crystal_density_diffrn    6.755
_cod_duplicate_entry             1007090
_cod_original_sg_symbol_H-M      'I 41/a'
_cod_database_code               9016210
_amcsd_formula_title             'Ge Hf O4'
The crystal chemistry and crystal structure of kuksite, Pb3Zn3Te6+P2O14, and a note on the crystal structure of yafsoanite, (Ca,Pb)3Zn(TeO6)2
Mills, S. J.; Kampf, A. R.; Kolitsch, U.; Housley, R. M.; Raudsepp, M.; American Mineralogist 95 (2010) 933–938; doi:10.2138/am.2010.3483

data_9016211
_publ_section_title
;
 The crystal chemistry and crystal structure of kuksite, Pb3Zn3Te6+P2O14,
 and a note on the crystal structure of yafsoanite, (Ca,Pb)3Zn(TeO6)2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              933
_journal_page_last               938
_journal_paper_doi               10.2138/am.2010.3483
_journal_volume                  95
_journal_year                    2010
_chemical_compound_source
'Black Pine mine, NW of Philipsburg, Granite County, Montana, USA'
_chemical_formula_sum            'As0.404 O14 P1.594 Pb3 Te Zn3'
_chemical_name_mineral           Kuksite
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   8.392
_cell_length_b                   8.392
_cell_length_c                   5.204
_cell_volume                     317.394
_database_code_amcsd             0005047
_exptl_crystal_density_diffrn    6.535
_cod_original_formula_sum        'Pb3 Te Zn3 P1.594 As.404 O14'
_cod_database_code               9016211
Effects of temperature and pressure on the crystal structure of ferromagnesian olivine T = 23 C, P = 1 atm , Evacuated silica capillary
Hazen, R. M.; American Mineralogist 62 (1977) 286–295; doi:

data_9016212
_publ_section_title
;
 Effects of temperature and pressure on the crystal structure of ferromagnesian
 olivine
 T = 23 C, P = 1 atm , Evacuated silica capillary
;
_journal_name_full               'American Mineralogist'
_journal_page_first              286
_journal_page_last               295
_journal_volume                  62
_journal_year                    1977
_chemical_compound_source        'Franklin, New Jersey, USA'
_chemical_formula_sum            'Fe1.1 Mg0.75 Mn0.15 O4 Si'
_chemical_name_mineral           Fayalite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.798
_cell_length_b                   10.390
_cell_length_c                   6.055
_cell_formula_units_Z            4
_cell_volume                     301.849
_database_code_amcsd             0000570
_exptl_crystal_density_diffrn    3.961
_cod_original_formula_sum        '(Fe1.1 Mg.75 Mn.15) Si O4'
_cod_database_code               9016212
High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction Note: P = 0 GPa, data from Ovsyannikov and Dubrovinsky (2011)
Kantor, A.; Kantor, I.; Merlini, M.; Glazyrin, K.; Prescher, C.; Hanfland, M.; Dubrovinsky, L.; American Mineralogist 97 (2012) 1764–1770; doi:10.2138/am.2012.4103

data_9016213
_publ_section_title
;
 High-pressure structural studies of eskolaite by means of single-crystal X-ray diffraction
 Note: P = 0 GPa, data from Ovsyannikov and Dubrovinsky (2011)
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1764
_journal_page_last               1770
_journal_paper_doi               10.2138/am.2012.4103
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Cr2 O3'
_chemical_name_mineral           Eskolaite
_space_group_crystal_system      trigonal
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.9530
_cell_length_b                   4.9530
_cell_length_c                   13.5884
_cell_volume                     288.693
_exptl_crystal_density_diffrn    5.245
_cod_depositor_comments
;
 Adding the _cell_formula_units_Z data item and updating the space group
 information.

 Antanas Vaitkus,
 2018-01-15
;
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_database_code               9016213
The plumose boulangerite from Bottino, Apuan Alps, Italy: Crystal structure, OD character and twinning Note: MDO1 polytype
Ventruti, G.; Stasi, F.; Pinto, D.; Vurro, F.; Renna, M.; The Canadian Mineralogist 50 (2012) 181–199; doi:10.3749/canmin.50.2.181

data_9016214
_publ_section_title
;
 The plumose boulangerite from Bottino, Apuan Alps, Italy:
 Crystal structure, OD character and twinning
 Note: MDO1 polytype
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              181
_journal_page_last               199
_journal_paper_doi               10.3749/canmin.50.2.181
_journal_volume                  50
_journal_year                    2012
_chemical_compound_source        'Bottino mine, Apuan Alps, Italy'
_chemical_formula_sum            'Pb10.15 S22 Sb7.85'
_chemical_name_mineral           Boulangerite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.76
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   21.554
_cell_length_b                   23.454
_cell_length_c                   8.079
_cell_volume                     4012.348
_database_code_amcsd             0019191
_exptl_crystal_density_diffrn    6.231
_cod_original_cell_volume        4012.349
_cod_original_formula_sum        'Pb10.15 Sb7.85 S22'
_cod_database_code               9016214
Uber Vaterit und seine Struktur
Meyer, H. J.; Angewandte Chemie 71 (1959) 678–679; doi:

data_9016215
_publ_section_title
;
 Uber Vaterit und seine Struktur
;
_journal_name_full               'Angewandte Chemie'
_journal_page_first              678
_journal_page_last               679
_journal_volume                  71
_journal_year                    1959
_chemical_formula_sum            'C Ca O3'
_chemical_name_mineral           Vaterite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.13
_cell_length_b                   7.15
_cell_length_c                   8.48
_cell_formula_units_Z            4
_cell_volume                     250.410
_database_code_amcsd             0019139
_exptl_crystal_density_diffrn    2.655
_cod_original_formula_sum        'Ca C O3'
_cod_database_code               9016215
Limitations of Fe2+ and Mn2+ site occupancy in tourmaline: Evidence from Fe2+ - and Mn2+ -rich tourmaline Note: sample mnelb3
Ertl, A.; Kolitsch, U.; Dyar, M. D.; Hughes, J. M.; Rossman, G. R.; Pieczka, A.; Henry, D. J.; Pezzotta, F.; Prowatke, S.; Lengauer, C. L.; Korner, W.; Brandstatter, F.; Francis, C. A.; Prem, M.; Tillmanns, E.; American Mineralogist 97 (2012) 1402–1416; doi:10.2138/am.2012.4028

data_9016216
_publ_section_title
;
 Limitations of Fe2+ and Mn2+ site occupancy in tourmaline:
 Evidence from Fe2+ - and Mn2+ -rich tourmaline
 Note: sample mnelb3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1402
_journal_page_last               1416
_journal_paper_doi               10.2138/am.2012.4028
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        'Elba, Italy'
_chemical_formula_sum
'Al7.767 B3 F0.57 H6 Mn1.233 Na0.666 O30.43 Si6'
_chemical_name_mineral           Fluor-tsilaisite
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   15.951
_cell_length_b                   15.951
_cell_length_c                   7.1380
_cell_formula_units_Z            3
_cell_volume                     1572.834
_database_code_amcsd             0019253
_exptl_crystal_density_diffrn    3.159
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum
'Na.666 Al7.767 Mn1.233 Si6 B3 F.57 O30.43 H6'
_cod_database_code               9016216
Spin-Glass Behavior in Sr2 Fe Ru O6 and Ba La Ni Ru O6: A Comparison with Antiferromagnetic Ba La Zn Ru O6 _cod_database_code 1001402
Battle, P.; Gibb, T.; Jones, C.; Studer, F.; Journal of Solid State Chemistry 78 (1989) 281–293; doi:10.1016/0022-4596(89)90109-6

data_9016217
_publ_section_title
;
 Spin-Glass Behavior in Sr2 Fe Ru O6 and Ba La Ni Ru O6: A
 Comparison with Antiferromagnetic Ba La Zn Ru O6
 _cod_database_code 1001402
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              281
_journal_page_last               293
_journal_paper_doi               10.1016/0022-4596(89)90109-6
_journal_volume                  78
_journal_year                    1989
_chemical_formula_sum            'Ba0.5 La0.5 Ni0.5 O3 Ru0.5'
_space_group_IT_number           2
_symmetry_space_group_name_Hall
'-P 1 (-1/2*x+1/2*y+1/2*z,1/2*x-1/2*y+1/2*z,1/2*x+1/2*y-1/2*z)'
_symmetry_space_group_name_H-M   'I -1'
_cell_angle_alpha                89.803
_cell_angle_beta                 90.10
_cell_angle_gamma                90.09
_cell_length_a                   5.5964
_cell_length_b                   5.5879
_cell_length_c                   7.9319
_cell_formula_units_Z            4
_cell_volume                     248.045
_database_code_amcsd             0013643
_exptl_crystal_density_diffrn    7.123
_cod_duplicate_entry             1001402
_cod_original_formula_sum        '(Ba.5 La.5) (Ni.5 Ru.5) O3'
_cod_database_code               9016217
_amcsd_formula_title             'Ba La Ni O6 Ru'
The single-crystal X-ray structures of bariopharmacosiderite-C, bariopharmacosiderite-Q and natropharmacosiderite Note: sample Bariopharmacosiderite-C
Hager, S. L.; Leverett, P.; Williams, P. A.; Mills, S. J.; Hibbs, D. E.; Raudsepp, M.; Kampf, A. R.; Birch, W. D.; The Canadian Mineralogist 48 (2010) 1477–1485; doi:10.3749/canmin.48.5.1477

data_9016218
_publ_section_title
;
 The single-crystal X-ray structures of bariopharmacosiderite-C,
 bariopharmacosiderite-Q and natropharmacosiderite
 Note: sample Bariopharmacosiderite-C
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1477
_journal_page_last               1485
_journal_paper_doi               10.3749/canmin.48.5.1477
_journal_volume                  48
_journal_year                    2010
_chemical_compound_source        'Robinson's Reef, Clunes, Victoria, Australia'
_chemical_formula_sum
'Al0.04 As2.16 Ba0.468 Fe3.96 H9.04 K0.039 Na0.021 O18.52 P0.84'
_chemical_name_mineral           Bariopharmacosiderite
_space_group_IT_number           215
_symmetry_space_group_name_Hall  'P -4 2 3'
_symmetry_space_group_name_H-M   'P -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   7.942
_cell_length_b                   7.942
_cell_length_c                   7.942
_cell_volume                     500.945
_database_code_amcsd             0019790
_exptl_crystal_density_diffrn    2.591
_cod_original_formula_sum
'Ba.468 K.039 Na.021 (Fe3.96 Al.04) O18.52 (As2.16 P.84) H9.04'
_cod_database_code               9016218
La structure cristalline de Rb2 Al F5, H2 O. Retour critique sur le type structural Tl2 Al F5 _cod_database_code 1000200
Fourquet, J.; Plet, F.; de Pape, R.; Revue de Chimie Minerale 18 (1981) 19–26; doi:

data_9016219
_publ_section_title
;
 La structure cristalline de Rb2 Al F5, H2 O. Retour critique sur
 le type structural Tl2 Al F5
 _cod_database_code 1000200
;
_journal_name_full               'Revue de Chimie Minerale'
_journal_page_first              19
_journal_page_last               26
_journal_volume                  18
_journal_year                    1981
_chemical_formula_sum            'Al F5 O Rb2'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   9.604
_cell_length_b                   8.379
_cell_length_c                   7.542
_cell_formula_units_Z            4
_cell_volume                     606.919
_database_code_amcsd             0015391
_exptl_crystal_density_diffrn    3.381
_cod_duplicate_entry             1000200
_cod_original_formula_sum        'Rb2 Al F5 O'
_cod_database_code               9016219
_amcsd_formula_title             'Al F5 H2 O Rb2'
Crystal structures of shlykovite and cryptophyllite: comparative crystal chemistry of phyllosilicate minerals of the mountainite family
Zubkova, N. V.; Filinchuk, Y. E.; Pekov, I. V.; Pushcharovsky, D. Y.; Gobechiya, E. R.; European Journal of Mineralogy 22 (2010) 547–555; doi:10.1127/0935-1221/2010/0022-2041

data_9016220
_publ_section_title
;
 Crystal structures of shlykovite and cryptophyllite: comparative crystal
 chemistry of phyllosilicate minerals of the mountainite family
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              547
_journal_page_last               555
_journal_paper_doi               10.1127/0935-1221/2010/0022-2041
_journal_volume                  22
_journal_year                    2010
_chemical_compound_source
'Mount Rasvumchorr, Khibiny alkaline intrusion, Kola Peninsula, Russia'
_chemical_formula_sum            'Ca H7 K O13 Si4'
_chemical_name_mineral           Shlykovite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 94.597
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.4897
_cell_length_b                   6.9969
_cell_length_c                   26.714
_cell_volume                     1209.121
_database_code_amcsd             0017556
_exptl_crystal_density_diffrn    2.233
_cod_original_formula_sum        'K Ca Si4 O13 H7'
_cod_database_code               9016220